x-ray photoelectron spectroscopy - nasa bide (mo2c), and titanium boride (tib2) were prepared for...
Post on 05-Jan-2020
Embed Size (px)
NASA Technical Paper 1033
>\ ASA TP 1033 c. 1
1 Spectroscopy ! Study of Radiofrequency-Sputtered Titanium Carbide, Molybdenum Carbide, and Titanium Boride Coatings and Their Friction Properties
William A. Brainard and Donald R. Wheeler
TECH LIBRARY KAFB, NM
NASA Technical Paper 1033
X-Ray Photoelectron Spectroscopy Study of Radiofrequency-Sputtered Titanium Carbide, Molybdenum Carbide, and Titanium Boride Coatings and Their Friction Properties
William A. Brainard and Donald R. Wheeler Lewis Research Center Cleveland, Ohio
National Aeronautics and Space Administration
Scientific and Technice’ Information Office
X-RAY PHOTOELECTRON SPECTROSCOPY STUDY OF RADIOFREQUENCY-
SPUTTERED TITANIUM CARBIDE, MOLYBDENUM CARBIDE, AND
TITANIUM BORIDE COATINGS AND THEIR FRICTION PROPERTIES
by Wi l l i am A. Bra inard and Dona ld R. Wheeler
Lewis Research Center
Radiofrequency (rf) sputtered coatings of titanium carbide (TIC), molybdenum car- bide (Mo2C), and titanium boride (TiB2) were prepared for friction and wear testing and analysis by X-ray photoelectron spectroscopy (XPS). Wear testing was conducted with a pin of 304 stainless steel on disk apparatus, the disks being type 440-C steel that were rf sputter coated. Emphasis was placed on correlating friction and wear data with bulk film properties, that is, stoichiometry and impurity content and, secondly, with interfacial adherence.
Titanium carbide coatings achieved maximum stoichiometry and minimum bulk film oxygen contamination when bias deposited at -500 volts. Adding 10 percent hydrogen to the plasma in an attempt to further reduce the level of oxygen contamination in poorly adherent films that failed during friction testing very quickly. Oxidizing the 440-C sub- strates prior to deposition produced marked improvements in friction and wear properties. The bulk composition of molybdenum carbide coatings w a s also improved by biasing (-300 V); however, biasing was detrimental to coating adherence. Bias deposited coat- ings would not adhere to sputter cleaned 440-C substrates flaking off due to internal film stresses even though a thick, graded interface (>2500 i.) was obtained. Films deposited in such a manner as to form an oxide at the interface adhered strongly even i f bias was subsequently employed to improve bulk film properties. Depth profile studies of two poorly adherent films showed little oxygen at the interface. Friction behavior of Mo2C films was either good or bad depending on whether or not oxide was formed at the inter- face during deposition.
Titanium boride coatings also exhibited a dependence on interfacial oxides to achieve maximum adherence. Friction and w e a r data are markedly improved by deliberately pre- oxidizing the substrate material.
These results suggest strongly that some of the commonly used practices in the deposition of these films, particularly rigorously precleaning substrates or sputtering without bias can be detrimental to the production of adherent, stoichiometric films for certain compounds and substrates.
In the field of friction and wear, there is considerable interest in the use of refrac- tory compound materials in bulk forms and as coatings such as in wire drawing dies o r foil bearings. Refractory compounds such as the molybdenum and titanium carbides, silicides and borides, are currently being investigated. The use of radiofrequency (rf) sputtering as a means of applying coatings of those materials is desirable for many rea- sons. Thin, dense coatings of a wide variety of materials including elemental metals, alloys, inorganic and organic compounds can be obtained on a wide variety of shapes and substrates without requiring high temperatures (ref. 1).
Previous work, however (ref. 2), has shown that the friction and wear behavior of rf sputtered films may not be satisfactory due to variations of stoichiometry, impurities, o r poor adherence. X-ray photoelectron spectroscopy (XPS) w a s used to examine several compound coatings applied by rf sputtering (ref. 3).
Those results indicated that significant bulk coating effects due to target history, sputtering time, power levels, and bias voltages could be observed. The friction and wear performance of sputtered films, however, depends not only on bulk film properties but is very much dependent on the interface, that is, the transition region between film and substrates. The bonding at the interface is crucial to the adherence behavior of the sputtered coatings and, thusly, the friction and wear performance.
The objective of this report is to present data on additional investigations on the nature of rf sputtered coatings with emphasis on the interface and the coating adherence. XPS analyses of sputtered coatings and interfaces were conducted in conjunction with deposition studies and pin on disk friction and wear tests. The materials examined were titanium carbide (Tic), titanium boride (TiB2), and molybdenum carbide (Mo2C). They were deposited on 440-C steel substrates.
APPARATUS AND PR0CEDUR;E
Radiofrequency Sputtering Apparatus
The sputtering of the materials used in this investigation was conducted in a com- mercial rf diode apparatus (fig. 1) operating at 13.56 megahertz. The material to be sputter deposited is in the form of a hot pressed compact which was commercially pur- chased. The specimen to be coated is placed 2.5 centimeters directly below the target on an electrically insulated block. An additional voltage from 0 to -1500 volts dc may be applied directly to the specimen either for specimen cleaning by dc sputter etching or for biasing the specimen during film deposition and growth. Provision is made for rotation
of the entire substrate table so the specimen may be moved out from under the target for cleaning. The target also can be cleaned in this manner without contaminating the specimen. The system is mechanically forepumped and oil diffusion pumped through a liquid nitrogen cooled baffle. During deposition, high purity argon (99.9995 percent) was bled continuously into the system through a leak valve and a dynamic pressure bal- ance between the pumping system and argon leak of approximately 20 microns was main- tained in the bell j a r .
Prior to actually starting deposition, the target was cleaned by rf sputtering until little pressure rise due to outgassing occurred. Following target cleaning, the rf was turned off. I€ desired, the specimen could then be also cleaned by dc sputter etching at -1200 volts for 15 minutes. Following specimen cleaning, the selected power and bias voltage parameters were set and the specimen rotated back under the target and deposi- tion initiated. Coatings thicknesses were 2000 to 3000 A except for the interface studies which were 400 to 500 A .
X-ray Photoelectron Spectroscopy
After deposition the films were analyzed by X-ray photoelectron spectroscopy (XPS). The principles of XPS are detailed in reference 4. X-ray photons striking an atom in the surface cause it to emit an electron. The electron will leave the atom with a kinetic energy K, which is the difference between the incident photon energy hv and the binding energy EB of the electron in the atom. The binding energy is characteristic of the atom excited and, in addition, depends slightly on the oxidation state of the atom. Thus, if the electron energies K emitted from a sample are measured and hv is known, the atoms in the sample may be identified and some chemical information extracted by comparing the measured binding energies with binding energies measured previously on standard samples. Because of the low kinetic energies (a keV) of the electrons, the atoms more than 20 A below the surface of a solid do not contribute to the spectrum.
The particular apparatus used here consisted of a commercial electron energy analyz- er and X-ray source in a vacuum system designed to accommodate a variety of samples. The system is a stainless steel bakeable ultrahigh vacuum system. It is ion pumped and incorporates a titanium sublimation pump. An ion gun in the system was used to gradually sputter away the sample surface and determine the composition as a function of depth. Details have been given previously (ref. 2). In addition, the system was provided with a gold coated tungsten filament that was used to evaporate a thin layer of gold onto the sample surface for calibration purposes.
Resolution of the spectral peaks is no less than 1.5 eV f u l l width at half maximum. The peak maxima can be located to &O. 1 eV at best. The energies are referenced to the
carbon (1s) line at 284.0 eV or the gold (4f ) peak at 84.0 eV and location of these lines adds *O. 2 eV to the absolute energy uncertainty. Therefore, *O. 3 eV is a rea- sonable estimate of the